- Nano Express
- Open Access
Photovoltaic Properties and Ultrafast Plasmon Relaxation Dynamics of Diamond-Like Carbon Nanocomposite Films with Embedded Ag Nanoparticles
© The Author(s). 2017
- Received: 30 December 2016
- Accepted: 11 April 2017
- Published: 20 April 2017
Ultrafast relaxation dynamics of diamond-like carbon (DLC) films with embedded Ag nanoparticles (DLC:Ag) and photovoltaic properties of heterojunctions consisting of DLC:Ag and crystalline silicon (DLC:Ag/Si) were investigated by means of transient absorption (TAS) spectroscopy and photovoltaic measurements. The heterojunctions using both p type and n type silicon were studied. It was found that TAS spectra of DLC:Ag films were dependent on the used excitation wavelength. At wavelengths where Ag nanoparticles absorbed light most intensively, only DLC signal was registered. This result is in good accordance with an increase of the DLC:Ag/Si heterojunction short circuit current and open circuit voltage with the excitation wavelength in the photovoltaic measurements. The dependence of the TAS spectra of DLC:Ag films and photovoltaic properties of DLC:Ag/Si heterostructures on the excitation wavelength was explained as a result of trapping of the photoexcited hot charge carriers in DLC matrix. The negative photovoltaic effect was observed for DLC:Ag/p-Si heterostructures and positive (“conventional”) for DLC:Ag/n-Si ones. It was explained by the excitation of hot plasmonic holes in the Ag nanoparticles embedded into DLC matrix. Some decrease of DLC:Ag/Si heterostructures photovoltage as well as photocurrent with DLC:Ag film thickness was observed, indicating role of the interface in the charge transfer process of photocarriers excited in Ag nanoparticles.
- Localized surface plasmon resonance
- Silver nanoparticles
- Photovoltaic properties
- Diamond-like carbon
- Electron-phonon interaction
- Charge transfer
- Hot electrons
- Magnetron sputtering
Nanostructures of IB group metals like Cu, Ag, and Au are interesting because of localized surface plasmon resonance (LSPR) effect . One of the prospective application areas for the plasmonics and plasmonic nanomaterials is photovoltaics where plasmonic nanostructures and metamaterials are used to control an interaction between light and solar cell. The increased optical path of light in solar cell as well as local increase of the absorption coefficient in vicinity of the plasmonic nanoparticle can be achieved [1, 2]. Recently, it was found that LSPR can be used for direct control of electrical properties of the solar cell. Plasmonic nanostructures, being in contact with the semiconductor, can either inject electrons into the semiconductor or trap electrons from the semiconductor as a result of the free charge carrier generation after interaction with the photons of the appropriate energy . Strong photovoltaic effect was observed for subbandgap photons of energy close to the LSPR energy of gold nanoparticles, when TiO2 substrate of the dye-sensitized (excitonic) solar cell (DSSC) was covered by non-percolating layer of Au nanoparticles . Such effect in principle can be applied for inorganic semiconductor (free charge carrier) solar cells, too. Till now, this effect was mostly studied for TiO2 covered by Au or Ag nanoparticles as well as Ag core shell nanoparticles covered by TiO2. However, the use of the nanoparticles synthesized by different wet chemical routes is not beneficial from the practical application point of view, i.e., because of the complications integrating this process into semiconductor device fabrication technologies. As an alternative approach to the fabrication methods mentioned above, deposition of metal and dielectric (semiconductor) nanocomposites by reactive magnetron sputtering or related physical vapor deposition-based methods could be considered. In such a way, metal nanoparticles embedded into the semiconductor or dielectric matrix can be grown during the same deposition process. In addition, dielectric or semiconducting matrix of the nanocomposite film with tunable refractive index can be used for the additional control of the optical properties of the plasmonic nanomaterial. Moreover, it can be applied to protect nanoparticles from unwanted environmental effects such as oxidation of Ag nanoparticles. It should be mentioned that Ag nanoparticles as a plasmonic material have some advantages over Au nanoparticles due to higher intensity of the LSPR , lower optical losses , and larger solar energy conversion efficiencies . However, silver nanoparticles are prone to rapid surface oxidation when exposed to ambient conditions . Thus, use of the plasmonic nanocomposite would eliminate the main advantage of Au over Ag—its chemical inertness. However, in such a case, one should look for other types of dielectric matrix because mostly used TiO2 as an oxide has some disadvantage as a matrix material. It is not able to efficiently protect embedded Ag nanoparticles from the oxidation [8, 9]. On the other hand, there are only few studies on plasmonic photoelectron excitation and emission in the systems containing semiconductor (or dielectric) material other than TiO2. Particularly, research on photovoltaic properties of the Ag core shell nanoparticles covered by oxide dielectric SiO2 [10, 11] as well as semiconducting oxide Fe2O3 thin layer on the top or beneath Au nanoparticles should be mentioned .
As one of the alternatives of matrix for Ag nanoparticles, amorphous diamond-like carbon (DLC) could be considered. DLC is an amorphous allotrope of carbon consisting of the sp2 bonded carbon nanoclusters embedded into the sp3 bonded carbon matrix. DLC is well known for its properties like high hardness, low friction, and chemical inertness as well as biocompatibility [13–16]. Refractive index, optical transmittance in a broad optical spectrum, including visible light and near IR ranges, and electrical properties of DLC films can be varied in a wide range choosing the deposition conditions. DLC films are deposited at room temperature by using a wide variety of the plasma based vacuum deposition processes that are compatible with the semiconductor device technology. This leads to different fields of applications such as optical windows, magnetic storage disks, bar code scanners, various mechanics, car parts, solid lubricants, biomedical coatings and micro-electromechanical devices [13, 15, 17], piezoresistive sensors [18–20], microwave switches , and electrically active high-power device passivation films . DLC matrix was proved as an excellent matrix for metal nanoparticles being able to prevent nanoparticles from chemical and mechanical hazards.
Considering photovoltaic properties of structures that include plasmonic nanoparticles, one should pay attention to the internal photoemission of the plasmonic hot electrons generated at the surface of the nanoparticles that is limited by hot electron recombination processes. Hot electron population usually decays due to the three main processes: thermalization of the electrons or in other words electron-electron scattering; electron-phonon interaction which describes hot (thermalized) electron energy transfer to the nanoparticle lattice; and finally, energy transfer from nanoparticle to the surrounding matrix. The process time scales are 10–100 fs, 0.1–5 ps, 1–100 ps, respectively [23–27]. These processes can become even more complex in the case of the nanoparticles embedded into the dielectric or semiconductor matrix.
This article aims at understanding of charge carrier generation, transfer and recombination processes in DLC films with embedded Ag nanoparticles (DLC:Ag nanocomposites), and role of these processes in the performance of photovoltaic properties of DLC:Ag/Si heterostructures. The analysis was performed by using transient absorption (TAS) spectroscopy and photovoltaic measurements. The unusual dependence of the TAS spectra of DLC:Ag films and photovoltaic properties of DLC:Ag/Si heterostructures on the excitation wavelength was found and explained.
Deposition of Thin Films and Heterostructures
In the present study, DLC:Ag films were deposited by direct current (DC) unbalanced magnetron sputtering of silver target. The diameter of magnetron was 3″. Polished polycrystalline alumina, monocrystalline silicon, and quartz substrates were used. Mixture of the hydrocarbons (acetylene) and argon gas was used in the reactive magnetron sputtering. In all experiments, substrate-target gap was set at 10 cm, magnetron target current was 0.1 A, base pressure was 5 ⋅ 10− 4 Pa and work pressure was (4 ± 1) 10−1 Pa. Samples were deposited on grounded substrates. Ar gas flux was 80 sccm and C2H2 gas flux was 7.8 sccm. As reported by our previous study , DLC:Ag films deposited using these conditions revealed the highest SERS signal intensity between all DLC films containing Ag investigated. Thus, strong plasmonic field can be supposed. According to our previous XPS measurement data, these films contained 22 at.% of Ag [19, 29] while average size of the Ag nanoclusters was ~10 nm . More information on chemical composition and structure of the samples can be found in [19, 29].
In most experiments, thickness of the films was 50 nm. To study the influence of the film thickness on the photovoltaic properties of the samples, film thickness was changed in 10–150 nm range.
Transient Absorption Measurements
The samples of DLC:Ag film on quartz were excited using ultrafast Yb:KGW laser Pharos (Light Conversion) with a regenerative amplifier generating 200 kHz repetition rate 290 fs duration pulses at 1030 nm wavelength. Avantes 2048 spectrophotometer was used for the steady-state absorption measurements. The proper excitation wavelength chosen from the highest absorption amplitude in the steady-state absorption spectra in most cases was tuned to 407, 470, 528, 627, and 736 nm with a collinear optical parametric generator Orpheus and harmonic generator Lyra (Light Conversion).
The samples of DLC:Ag film on quartz were probed with a white light supercontinuum generated using 2-mm-thick sapphire plate excited with the fundamental laser wavelength at 1030 nm. The spectral range of supercontinuum as well as the detection range of the TAS spectra dynamics was from 480 to 1000 nm. The excitation beam was focused to a spot of about 700 μm in diameter, while the probe white light supercontinuum beam diameter was of about 500 μm. Further details on the optical setup used can be found elsewhere .
OriginPro 2015 was used for the exponential and bi-exponential decay fitting of the TAS spectra.
Optical Properties of DLC:Ag Nanocomposites
Steady-State Optical Properties of DLC:Ag Nanocomposites
First of all, optical absorption spectra of DLC:Ag nanocomposite as well as DLC matrix used should be described; therefore, pure DLC and DLC:Ag steady-state absorption spectra are presented in Fig. 2. The absorption peak at about 470 nm is attributed to the LSPR absorption, while increase of the absorption at 300 nm and lower wavelengths is related to the absorption in DLC matrix . One can see that absorption due to DLC matrix above 600 nm becomes negligible.
Dynamic Optical Properties of Pure DLC Matrix
One can see that the TAS spectra of DLC matrix consist of positive signal in all measured spectral region (Fig. 3a). This signal can be attributed to the signal of induced absorption. In the region of the shortest wavelengths (below 500 nm), the positive signal decreases significantly showing that different processes take place which we can attribute to the ground-state bleaching .
Careful analysis of the TAS spectra dynamics (Fig. 3b) revealed that the curves of relaxation of pure DLC matrix for the all used excitation wavelengths consist of two components. Using bi-exponential decay function, the relaxation times of DLC matrix were revealed which are 0.41 ± 0.02 ps and 6.39 ± 0.45 ps, respectively, (decay kinetics at 600 nm was used for fitting because of the least noise and highest amplitude signal in this region).
Dynamic Optical Properties of DLC:Ag Nanocomposites
TAS spectra dynamics show clear dependence on the wavelength of excitation, e.g., DLC:Ag nanocomposites excited at 406, 470, and 528 nm show only positive signal in all spectra region, except dramatic amplitude decrease below 500 nm. The origin of this decrease may be similar to the pure DLC matrix.
Sample of DLC:Ag excited at higher wavelengths of 627 and 736 nm shows strong, short-living negative signal. The relaxation of this signal is much faster than that of the positive one. The lifetime of this signal suggests that it could be attributed to LSPR relaxation, and the process called electron-phonon interaction is responsible for this short decay .
Lifetimes of TAS spectra relaxation (the kinetics at 600 nm probe wavelengths are presented because they demonstrate best SNR)
Excitation wavelength (nm)
Probe wavelength (nm)
τ 1 (ps)
τ 2 (ps)
0.41 ± 0.02
6.39 ± 0.45
0.75 ± 0.09
6.11 ± 0.60
0.70 ± 0.06
7.36 ± 0.48
0.36 ± 0.04
0.22 ± 0.03
No phonon-phonon interaction was registered. Probably, TAS signal of DLC overruns this signal, which should have quite low intensity . After less than 0.5 ps, the negative signal decays and transforms to the long-lived positive signal, which can be attributed to DLC matrix TAS signal. This approach allows to explain TAS signal of DLC:Ag after excitation at 627 and 736 nm, but unfortunately, it does not explain so well DLC:Ag relaxation signal after excitation at 406, 470, and 528 nm wavelengths, despite the fact that Ag nanoparticles in this spectral region should absorb light more intensively (Fig. 2).
The main peculiarity of these spectral data (406, 470, and 528 nm excitation) is an absence of the negative signal and high-relaxation lifetime that appears too long for the relaxation of plasmons. In fact, these TAS spectra are much more similar to the ones recorded for pure DLC matrix signal than to the LSPR of Ag nanoparticles relaxation dynamics. One could suppose that only DLC matrix is excited in this area, but the steady-state absorption spectra in Fig. 2 show different data (the intense absorption peak of DLC:Ag nanocomposites is at around 470 nm). While the absorption of DLC matrix and DLC:Ag nanocomposites is comparable at 406 nm, absorption by Ag nanoparticles at 470 nm should be larger than that by DLC matrix. Nevertheless, the TAS signal of DLC matrix completely overruns the signal of LSPR of Ag nanoparticles. This probably can be explained by interaction between the DLC matrix and Ag nanoparticles as charge transfer from Ag nanoparticles to DLC matrix, although it should be a very fast process because we were not able to distinguish it in the TAS relaxation dynamics.
We have also compared the relaxation decay times of DLC:Ag nanocomposites excited at 406 and 470 nm with the ones of pure DLC matrix. Fitting by the bi-exponential decay function shows that relaxation times of the “slow” relaxation component for DLC:Ag films (excited by 406 and 470 nm) are very similar to ones of the DLC matrix, showing that all these three TAS spectra represent the dynamics of DLC matrix (Table 1). Slow relaxation component disappears in the case of the DLC:Ag film TAS spectra excited by higher wavelength light (627 and 736 nm). Thus, it can be supposed that this component is related with processes in DLC matrix (Table 1). Relaxation dynamics of the positive signal consists of two components “fast” (τ 1) and slow (τ 2). The negative signal relaxation has only fast relaxation term in the negative area. That is why, only this component of relaxation time was explored. TAS signal changes fast from the negative to long-living positive signal. In order not to increase confusion, only relaxation time of short-living negative signal was included into Table 1.
Photovoltaic Properties of DLC:Ag/Si Heterostructures
According to Fig. 6a, b, open circuit voltage and short circuit current increase with the excitation wavelength. Such a behavior is a bit unexpected, as in numerous studies on generation of the plasmonic hot carriers, the conversion efficiency of incident photon to current was highest when the excitation wavelength was equal to the plasmonic absorbance peak wavelength [3, 10, 11, 35–41].
Analyzing photovoltaic properties of the studied heterostructures, one can see negative photovoltaic effect in the case of DLC:Ag/p-Si heterostructures. While for the DLC:Ag/n-Si heterostructures, positive (“conventional”) photovoltaic effect was registered. It should be mentioned that negative photovoltaic effect and negative open circuit voltage were reported in the case of some plasmonic nanostructures [42–44]. Particularly, visible plasmon irradiation of citrate coated Ag nanoparticles resulted in photogeneration of the negative photovoltage [42, 43]. It was explained by citrate photooxidation by Ag plasmon “hot holes” . The negative photovoltage was observed for some ZnO:Al/SiO2/p-Si structures, when 1740–1925 nm wavelength light was used for excitation , while positive (conventional) photovoltaic effect was detected for 560 nm wavelength excitation. Thus, observed negative photovoltaic effect in DLC:Ag/p-Si heterostructure is mainly related to the DLC:Ag film. As for DLC/p-Si heterojunctions, only positive (conventional) photovoltaic effect was reported (see e.g., [45, 46]), one could suggest that some LSPR-related hot carrier generation processes took place in our experiment. Plasmonic photoexcitation of the hot holes can be supposed. This process should clearly prevail over excitation of the plasmonic hot electrons. It should be mentioned that according to the theoretical study presented in , in the case of Ag at some excitation wavelengths, only hot holes are collected and no electrons.
No clear dependence of the DLC:Ag/Si heterostructures photovoltage and photocurrent on DLC:Ag film thickness was found in 10–50 nm range, while meaningful decrease of photovoltage and photocurrent was observed for the DLC:Ag films with thickness of 150 nm. This effect was observed despite strong dependence of the absorbance of the DLC:Ag films on thickness. It seems that photoemission of the plasmonic charge carriers to the silicon takes place only from a very thin DLC:Ag layer that is close to the DLC:Ag/Si interface. Taking into account the data presented in Fig. 7 and discussions above, it can be supposed that in our case, average mean free path of the charge carriers photoemitted from Ag nanoparticles is clearly no more than the smallest thickness of the DLC:Ag films studied in this article, i.e., −10 nm. It should be mentioned that in , we have shown that the Ag nanoparticle size in DLC was 5–10 nm according to TEM, while according to the AFM data, most often, Ag nanoparticle size was ~10 nm. According to Fig. 4, the negative absorbance peaks, representing photogeneration of the plasmonic charge carriers, disappears in ~0.5 ps. Thus, it seems that due to the fast recombination of the photoelectrons, photoemission mostly takes place from the Ag nanoparticles, which are in close vicinity with the DLC:Ag/Si interface. However, taking into account the influence of the interaction between DLC matrix and Ag nanoparticles at lower excitation wavelength, it can be supposed that most of the photoelectrons reach silicon via ultrathin interlayer of DLC. Thus, it seems that recombination or trapping of the photoexcited charge carriers in DLC matrix takes place. Plasmonic photocarriers excited in Ag nanoparticles, which are located too far from the DLC:Ag/Si interface are unable to reach silicon. Decrease of the photovoltaic parameters with the increase of the DLC:Ag film thickness up to 50 nm can be explained by effects of the increased light absorption in the film. Less photons reach the DLC:Ag film zone near the interface with Si. Finally, it results in the decreased photocurrent and photovoltage.
Correlation between the optical absorbance spectra excited by different wavelength light and respective photovoltaic characteristics of the samples can be identified. Particularly, TAS spectra excited by 406–528 nm light are much more similar to the ones recorded for pure DLC matrix signal than to LSPR of Ag nanoparticles relaxation dynamics. Only in the case of the samples excited by 627 and 736 nm, the negative absorption signal, e.g., generation of the hot charge carriers can be seen. Such behavior was found despite that maximum of the plasmonic absorption peak was observed at ~500 nm. On the other hand, open circuit voltage and short circuit current of the samples clearly increased with the excitation wavelength. Such tendency was observed despite the decreased lifetime of the photoexcited charge carriers measured by TAS (see τ1 in Table 1). Thus, according to Table 1, decrease of the photovoltaic parameters with the excitation wavelength should be expected, as higher photoexcited charge carrier lifetime results in the increased short circuit current. Yet, in our case, the reverse tendency is observed. It seems that at lower excitation, wavelength influence of the DLC matrix results in suppression of the surface plasmon resonance-related hot charge carrier photogeneration. Alternatively, one can suppose that insertion of Ag nanoclusters into the DLC matrix results in the rearrangement of the density of the states (DOE). Particularly in , it was shown that in some cases, hot carrier collection efficiencies are higher in the case of 700 and 1500 nm excitation wavelengths in comparison with the higher energy 400 nm wavelength photons.
It should be mentioned that in numerous studies, hot charge carrier generation or photovoltaic quantum efficiency spectra correlate with the absorption spectra of the plasmonic absorber. In most mentioned studies, Ag or Au nanoparticles (nanostructures) were embedded into the wide bandgap semiconductor TiO2 or were at the interface with TiO2. However, it seems that quantum efficiency spectra of Au nanostructure/Si junctions follow this approach, too . Only in , some similarities with the present study were observed, where deposition of Au nanoparticles on the magnetron-sputtered amorphous silicon film resulted in the increased photocurrent in 600–1000 nm range as well as increase of the photocurrent enhancement with photon wavelength in 450–1000 nm range with increased photon wavelength. No clear correlation between the changes of the photocurrent spectra and absorbance spectra of the plasmonic nanostructures was found in . In , no correlation between the negative photovoltage excited in Ag nanoparticle and citrate system by different wavelength light and Ag nanoparticle optical absorption spectra was found, too. However, in , negative photovoltage increased with exciting photon energy. While in the present study, photovoltage decreased with the exciting photon energy.
The tendencies observed in this research can be explained by taking into account possible influence of the traps. The results reported in  should be mentioned as well. Negative photoconductivity was also observed for InAs nanowires . Origin of the negative photoconductivity was attributed to the depletion of conduction channels by light-assisted hot-electron trapping . Photoconductivity lowering was excitation wavelength dependent. Photocurrent decreased more when excitation wavelength was shorter (higher photon energy) . In our case, we can suppose that at high excitation energies trapping of the hot charge carriers in DLC matrix or at the Ag nanoparticle/DLC interface takes place. Thus, photoexcitation of the plasmonic charge carriers competes with the trapping process. It results in suppression of the bleaching in DLC:Ag transient spectra excited by higher energy photons as well as decreased photocurrent and photovoltage. Energy of the hot charge carriers excited by longer wavelength photons is below trap-related states. In such a case, photoexcited plasmonic charge carriers avoid trapping. It results in the increased sample’s photocurrent and photovoltage at higher excitation wavelengths. This fact correlates with the TAS measurements when in TAS spectra of DLC:Ag films excited at higher wavelengths of 627 and 736 nm strong negative signal was observed, too.
We suppose that after excitation of the samples with shorter wavelengths (406–528 nm), charge transfer efficiency overruns hot electron relaxation. That is why we do not observe dynamics that we can attribute to LSPR relaxation, and DLC matrix signal dominates in the TAS spectra. While at longer wavelengths (627 and 736 nm), LSPR relaxation is much more effective process and we can see it clearly in the signal. From the first look, the photovoltaic characteristics should be better when excitation at shorter wavelengths is applied, but high-energy defects in the DLC matrix trap charges and reverse photovoltaic dependencies on the excitation wavelength completely. It is worth to mention that in some cases of plasmonic nanomaterials, photoexcitation of the charge carrier is more efficient at higher wavelengths. Particularly, under excitation at longer wavelengths (~700 nm), free electrons and holes can be generated in Ag nanoparticles while at shorter wavelengths (~400 nm), only generation of holes is effective .
In conclusion, hot plasmonic holes were excited in Ag nanoparticles embedded into the DLC matrix. Therefore, negative photovoltaic effect was observed for DLC:Ag/p-Si heterostructures and conventional positive for DLC:Ag/n-Si ones. Some decrease of the DLC:Ag/Si heterostructures photovoltage and photocurrent with DLC:Ag film thickness was found in 10–150 nm range. It means that photocarriers excited in the Ag nanoparticles, which are located too far from the DLC:Ag/Si interface, are unable to reach silicon due to the recombination. The dependence of the TAS spectra of DLC:Ag films and photovoltaic properties of DLC:Ag/Si heterostructures on the excitation wavelength can be explained by trapping of the hot charge carriers in DLC matrix. This process prevailed over plasmonic photogeneration of the hot charge carriers at lower excitation wavelengths, while energy of the hot charge carrier’s photoexcited by longer wavelength photons was lower than the energy of the trap states. Therefore, these lower energy carriers avoided trapping by DLC defects.
This research was funded by the European Social Fund under the Global Grant measure (project no. VP1-3.1-ŠMM-07-K-03-057).
ŠM planned the experiments and has been involved in writing and drafting the manuscript. AV and AČ prepared the samples and researched the photovoltaic properties. RG investigated the photovoltaic properties. DP and TT researched the ultrafast relaxation dynamics. IY has been involved in writing and arranging the manuscript. ST critically revised the manuscript and added important intellectual content. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Osgood R, Cao L, Panoiu N, Fan W, Zhang S, Malloy K, Brueck S (2009) Nonlinear plasmonics. Nat Photonics 6:737–748Google Scholar
- Warren SC, Walker DA, Grzybowski BA (2012) Plasmoelectronics: coupling plasmonic excitation with electron flow. Langmuir 28:9093–9102View ArticleGoogle Scholar
- Mubeen S, Hernandez-Sosa G, Moses D, Lee J, Moskovits M (2011) Plasmonic photosensitization of a wide band gap semiconductor: converting plasmons to charge carriers. Nano Lett 11:5548–5552View ArticleGoogle Scholar
- Peña-Rodríguez O, Pal U (2011) Enhanced plasmonic behavior of bimetallic (Ag-Au) multilayered spheres. Nanoscale Res Lett 6:279View ArticleGoogle Scholar
- West PR, Ishii S, Naik GV, Emani NK, Shalaev VM, Boltasseva A (2010) Searching for better plasmonic materials. Laser Photon Rev 4:795–808View ArticleGoogle Scholar
- Wang F, Melosh NA (2011) Plasmonic energy collection through hot carrier extraction. Nano Lett 11:5426–5430View ArticleGoogle Scholar
- Formo EV, Mahurin SM, Robust DS, SERS (2010) Substrates generated by coupling a bottom-up approach and atomic layer deposition. ACS Appl Mater Interfaces 2:1987–1991View ArticleGoogle Scholar
- Awazu K, Fujimaki M, Rockstuhl C, Tominaga J, Murakami H, Ohki Y, Yoshida N, Watanabe T (2008) A plasmonic photocatalyst consisting of silver nanoparticles embedded in titanium dioxide. J Am Chem Soc 130:1676–1680View ArticleGoogle Scholar
- Zhang H, Wang G, Chen D, Lv X, Li J (2008) Tuning photoelectrochemical performances of Ag−TiO2 nanocomposites via reduction/oxidation of Ag. Chem Mater 20:6543–6549View ArticleGoogle Scholar
- Reineck P, Lee GP, Brick D, Karg M, Mulvaney P, Bach U (2012) A solid-state plasmonic solar cell via metal nanoparticle self-assembly. Adv Mater 24:4750–4755View ArticleGoogle Scholar
- Brown MD, Suteewong T, Kumar RSS, Innocenzo VD, Petrozza A, Lee MM, Wiesner U, Snaith HJ (2011) Plasmonic dye-sensitized solar cells using core-shell metal-insulator nanoparticles. Nano Lett 11:438–445View ArticleGoogle Scholar
- Thimsen E, Le Formal F, Grätzel M, Warren SC (2011) Influence of plasmonic Au nanoparticles on the photoactivity of Fe2O3 electrodes for water splitting. Nano Lett 11:35–43View ArticleGoogle Scholar
- Robertson J (2008) Comparison of diamond-like carbon to diamond for applications. Phys Status Solidi Appl Mater Sci 205:2233–2244View ArticleGoogle Scholar
- Robertson J (2002) Diamond-like amorphous carbon. Mater Sci Eng R Reports 37:129–281View ArticleGoogle Scholar
- Schall JD, Gao G, Harrison JA (2010) Effects of adhesion and transfer film formation on the tribology of self-mated DLC contacts. J Phys Chem C 114:5321–5330View ArticleGoogle Scholar
- Hayashi K, Tezuka K, Ozawa N, Shimazaki T, Adachi K, Kubo M (2011) Tribochemical reaction dynamics simulation of hydrogen on a diamond-like carbon surface based on tight-binding quantum chemical molecular dynamics. J Phys Chem C 115:22981–22986View ArticleGoogle Scholar
- Santra TS, Bhattacharyya TK, Patel P, Tseng FG, Barik TK. (2012). Diamond, diamond-like carbon (DLC) and diamond-like nanocomposite (DLN) thin films for MEMS applications, microelectromechanical systems and devices, Dr Nazmul Islam (Ed.), ISBN: 978-953-51-0306-6, InTech, Available from: http://www.intechopen.com/books/microelectromechanical-systems-and-devices/diamonddiamond-like-carbon-dlc-and-diamond-like-nanocomposite-dln-thin-films-for-memsapplications-
- Petersen M, Heckmann U, Bandorf R, Gwozdz V, Schnabel S, Bräuer G, Klages CP (2011) Me-DLC films as material for highly sensitive temperature compensated strain gauges. Diam Relat Mater 20:814–818View ArticleGoogle Scholar
- Meškinis S, Vasiliauskas A, Šlapikas K, Gudaitis R, Andrulevičius M, Čiegis A, Niaura G, Kondrotas R, Tamulevičius S (2014) Bias effects on structure and piezoresistive properties of DLC: Ag thin films. Surf Coatings Technol 255:84–89View ArticleGoogle Scholar
- Uhlig S, Schmid-Engel H, Speicher T, Schultes G (2013) Pressure sensitivity of piezoresistive nickel-carbon Ni:a-C:H thin films. Sensors Actuators A Phys 193:129–135View ArticleGoogle Scholar
- Bhattacharyya S, Henley SJ, Mendoza E, Gomez-Rojas L, Allam J, Silva SRP (2006) Resonant tunnelling and fast switching in amorphous-carbon quantum-well structures. Nat Mater 5:19–22View ArticleGoogle Scholar
- Barthelmes R, Beuermann M, Metzner D, Winter N, Reznik D (1998) Electroactive passivation of high power semiconductor devices with punch through design by hydrogenated amorphous carbon layers (aC:H). Proc 1998 Intemational Symp Power Semicond Devices ICs, Kyoto, pp 181–184Google Scholar
- Bigot J-Y, Halté V, Merle J-C, Daunois A (2000) Electron dynamics in metallic nanoparticles. Chem Phys 251:181–203View ArticleGoogle Scholar
- You G-J, Zhou P, Zhang C-F, Dong Z-W, Yang F, Du Z-L, Chen L-Y, Qian S-X (2005) Ultrafast studies on the energy relaxation dynamics and the concentration dependence in Ag:Bi2O3 nanocomposite films. Chem Phys Lett 413:162–167View ArticleGoogle Scholar
- Jain PK, Qian W, El-Sayed MA (2006) Ultrafast electron relaxation dynamics in coupled metal nanoparticles in aggregates. J Phys Chem B 110:136–42View ArticleGoogle Scholar
- Huang W, Qian W, El-Sayed MA, Ding Y, Wang ZL (2007) Effect of the lattice crystallinity on the electron-phonon relaxation rates in gold nanoparticles. J Phys Chem C 111:10751–10757View ArticleGoogle Scholar
- Darugar Q, Qian W, El-Sayed MA, Street S, Pileni M, Marie P (2006) Size-Dependent Ultrafast Electronic Energy Relaxation and Enhanced Fluorescence of Copper Nanoparticles. J Phys Chem B 110:143–149View ArticleGoogle Scholar
- Meškinis Š, Tamulevičius T, Niaura G, Šlapikas K, Vasiliauskas A, Ulčinas O, Tamulevičius S (2016) Surface enhanced raman scattering effect in diamond like carbon films containing Ag nanoparticles. J Nanosci Nanotechnol 16:10143–10151View ArticleGoogle Scholar
- Čiegis A, Vasiliauskas A, Tamulevičienė A, Niaura G, Tamulevičius S (2014) Plasmonic properties of silver nanoparticles embedded in diamond like carbon films: influence of structure and composition. Appl Surf Sci 317:1041–1046View ArticleGoogle Scholar
- Yaremchuk I, Meškinis Š, Fitio V, Bobitski Y, Šlapikas K, Čiegis A, Balevičius Z, Selskis A, Tamulevičius S (2015) Spectroellipsometric characterization and modeling of plasmonic diamond-like carbon nanocomposite films with embedded Ag nanoparticles. Nanoscale Res Lett 10:157View ArticleGoogle Scholar
- Peckus D, Tamulevičius T, Meškinis Š, Tamulevičienė A, Vasiliauskas A, Ulčinas O, Gulbinas V, Tamulevičius S (2016) Linear and nonlinear absorption properties of diamond-like carbon doped with Cu nanoparticles. Plasmonics. doi: 10.1007/s11468-016-0227-0
- Berera R, Grondelle R, Kennis JTM (2009) Ultrafast transient absorption spectroscopy: principles and application to photosynthetic systems. Photosynth Res 101:105–118View ArticleGoogle Scholar
- Lysenko S, Jimenez J, Zhang G, Liu H (2006) Nonlinear optical dynamics of glass-embedded silver nanoparticles. J Electron Mater 35:1715–1721View ArticleGoogle Scholar
- Juvé V, Scardamaglia M, Maioli P, Crut A, Merabia S, Joly L, Del Fatti N, Vallée F (2009) Cooling dynamics and thermal interface resistance of glass-embedded metal nanoparticles. Phys Rev B 80:195406View ArticleGoogle Scholar
- Lee YK, Lee H, Park JY. Tandem-structured, hot electron based photovoltaic cell with double Schottky barriers. Sci Rep. 2014;4:4580Google Scholar
- Manjavacas A, Liu JG, Kulkarni V, Nordlander P.Plasmon-Induced Hot Carriers in Metallic Nanoparticles. ACS Nano. 2014;8:7630–7638Google Scholar
- Zhukovsky SV, Babicheva VE, Uskov AV, Protsenko IE, Lavrinenko AV. Enhanced electron photoemission by collective lattice resonances in plasmonic nanoparticle-array photodetectors and solar cells. Plasmonics. 2014;9:283–289 Google Scholar
- Takahashi Y, Tatsuma T. Solid state photovoltaic cells based on localized surface plasmon-induced charge separation. Appl Phys Lett. 2011;99:182110Google Scholar
- Nishijima Y, Ueno K, Yokota Y, Murakoshi K, Misawa H. Plasmon-assisted photocurrent generation from visible to near-infrared wavelength using a au-nanorods/TiO2 electrode. J Phys Chem Lett. 2010;1:2031–2036Google Scholar
- Lee J, Mubeen S, Ji X, Stucky GD, Moskovits M. Plasmonic photoanodes for solar water splitting with visible light. Nano Lett. 2012;12:5014−5019Google Scholar
- Lee YK, Jung CH, Park J, Seo H, Somorjai GA, Park JY. Surface plasmon-driven hot electron flow probed with metal-semiconductor nanodiodes. Nano Lett. 2011;11:4251–4255Google Scholar
- Wu X, Redmond PL, Liu H, Chen Y, Steigerwald M, Brus L. Photovoltage mechanism for room light conversion of citrate stabilized silver nanocrystal seeds to large nanoprisms. J Am Chem Soc. 2008;130:9500–9506Google Scholar
- Thrall ES, Steinberg AP, Wu X, Brus LE. The role of photon energy and semiconductor substrate in the plasmon-mediated photooxidation of citrate by silver nanoparticles. J Phys Chem C. 2013;117:26238–26247Google Scholar
- Pradhan AK, Holloway T, Mundle R, Dondapati H, Bahoura M. Energy harvesting in semiconductor-insulator-semiconductor junctions through excitation of surface plasmon polaritons. Appl Phys Lett. 2012;100:1–4Google Scholar
- Rusop M, Ebisu H, Adachi M, Soga T, Jimbo T. Physical and microstructural properties of radio-frequency plasma-enhanced chemical vapor deposition grown n-type phosphorus doped amorphous carbon films on the contribution to carbon-based solar cells. Jpn J Appl Phys. 2005;44:6124Google Scholar
- Tian X, Soga T, Jimbo T, Umeno M. The a-C:H/p-Si solar cell deposited by pulsed laser deposition. J Non Cryst Solids. 2004;336:32–36Google Scholar
- Gong T, Munday JN. Materials for hot carrier plasmonics. Opt Mater Express. 2015;5:56–62Google Scholar
- Trevino J, Forestiere C, Di Martino G, Yerci S, Priolo F, Dal Negro L. (2012) Plasmonic-photonic arrays with aperiodic spiral order for ultra-thin film solar cells. Optics Express. 20(S3):A418Google Scholar
- Yang Y, Peng X, Kim HS, Kim T, Jeon S, Kang HK, Choi W, Song J, Doh YJ, Yu D. (2015) Hot Carrier Trapping Induced Negative Photoconductance in InAs Nanowires toward Novel Nonvolatile Memory. Nano Letters.15(9):5875-5882Google Scholar